# Machine Learning-Assisted High-Throughput Molecular Dynamics Simulation of High-Mechanical Performance Carbon Nanotube Structure

^{1}

^{2}

^{3}

^{*}

## Abstract

**:**

## 1. Introduction

^{3}interwall bonding, Xia et al. [19] found that the interwall sp

^{3}coupling in MWCNTs enhanced the load transfer among the walls, facilitating their complete mechanical participation; this prevented the telescoping problem during tensile testing and improved the MWCNT strength. Alternately, Peng et al. [15] reported that the fracture strength value of MWCNTs treated with controlled electron irradiation could reach as high as 80% of the value expected in defect-free SWCNTs; this is considered to be the result of crosslinking between the walls. They further confirmed through molecular mechanics approaches that the interwall load transfer improves on increasing Frenkel-pair-type crosslinks, and only a small percentage of these crosslinks is necessary to achieve optimal load transfer. In contrast with their experiment [15], the MD results obtained by Byrne et al. [20] showed that defective MWCNTs with sp

^{3}interwall bonding exhibited strength values exceeding those of SWCNTs (of the same size) with crack-like defects, and concluded that composites with suitably designed MWCNTs would perform better than most SWCNT-based composites. Furthermore, Shirasu et al. [18] performed theoretical calculations and experiments to prove that the nominal tensile strength is the key factor in determining the mechanical properties when designing CNT-reinforced composites, rather than the effective tensile strength. The effective tensile strength is given by the total force divided by the area that bears the load, while the nominal tensile strength is given by the total force divided by the total area, including the hollow core. It is also highlighted in the study [18] that an effective method to improve the nominal tensile strength is to introduce crosslinks between the MWCNT walls.

## 2. Molecular Dynamics Models and Computational Methods

^{9}s

^{−1}and time step at 0.5 fs. Please note that the fixed part also experienced elongation along the tube axis as the load increased, while all the atoms in the mobile part including the middle portion of the outermost wall and all inner walls could move freely, as shown in Figure 1. To avoid non-physical increases in stress values during tensile loading, the AIREBO potential cutoff distance was modified to 2.0 Å [27,28,29]. The resultant tensile strength of the AIREBO potential–based tensile test verification simulation of the zigzag-type CNTs obtained in this study was 120 GPa. This was slightly higher than the experimental result, and consistent with those of the quantum calculation obtained by B. Peng et al. [15], which were approximately 100 GPa and 120 GPa. Moreover, the strain-stress relation for single-walled fracture of MWCNTs was in good agreement with their experiment sample 1, 2 and 3. Because the distribution pattern of the crosslinks may influence the result and the interwall crosslink density has at most 3% margin of error after equilibration, at least three calculations were performed for each MWCNT model, and the average values were considered to be the final results.

^{®}SOMine 5.2.2 Expert Edition [43], was employed to produce SOMs. In addition to the general SOM algorithm, a Kohonen’s batch map based on an advanced unsupervised neural network [44] was deployed inside the software. For parameters in SOM, the number of nodes and topology were set to 1000 and hexagonal, respectively.

## 3. Results

## 4. Discussion

## 5. Conclusions

## Author Contributions

## Funding

## Acknowledgments

## Conflicts of Interest

## References

- Iijima, S. Helical microtubules of graphitic carbon. Nature
**1991**, 354, 56–58. [Google Scholar] [CrossRef] - Bakshi, S.R.; Lahiri, D.; Agarwal, A. Carbon nanotube reinforced metal matrix composites—A review. Int. Mater. Rev.
**2010**, 55, 41–64. [Google Scholar] [CrossRef] - Ozaki, T.; Iwasa, Y.; Mitani, T. Stiffness of single-walled carbon nanotubes under large strain. Phys. Rev. Lett.
**2000**, 84, 1712. [Google Scholar] [CrossRef][Green Version] - Ogata, S.; Shibutani, Y. Ideal tensile strength and band gap of single-walled carbon nanotubes. Phys. Rev. B
**2003**, 68, 165409. [Google Scholar] [CrossRef] - Troya, D.; Mielke, S.L.; Schatz, G.C. Carbon nanotube fracture–differences between quantum mechanical mechanisms and those of empirical potentials. Chem. Phys. Lett.
**2003**, 382, 133–141. [Google Scholar] [CrossRef] - Zhang, Y.; Iijima, S.; Shi, Z.; Gu, Z. Defects in arc-discharge-produced single-walled carbon nanotubes. Philos. Mag. Lett.
**1999**, 79, 473–479. [Google Scholar] [CrossRef] - Zhang, S.; Mielke, S.L.; Khare, R.; Troya, D.; Ruoff, R.S.; Schatz, G.C.; Belytschko, T. Mechanics of defects in carbon nanotubes: Atomistic and multiscale simulations. Phys. Rev. B
**2005**, 71, 115403. [Google Scholar] [CrossRef] - Tserpes, K.I.; Papanikos, P. The effect of Stone-Wales defect on the tensile behavior and fracture of single-walled carbon nanotubes. Compos. Struct.
**2007**, 79, 581–589. [Google Scholar] [CrossRef] - Suenaga, K.; Wakabayashi, H.; Koshino, M.; Sato, Y.; Urita, K.; Iijima, S. Imaging active topological defects in carbon nanotubes. Nat. Nanotechnol.
**2007**, 2, 358–360. [Google Scholar] [CrossRef] - Xia, Z.; Riester, L.; Curtin, W.A.; Li, H.; Sheldon, B.W.; Liang, J.; Chang, B.; Xu, J.M. Direct observation of toughening mechanisms in carbon nanotube ceramic matrix composites. Acta Mater.
**2004**, 52, 931–944. [Google Scholar] [CrossRef] - Zhou, Z.; Wang, S.; Lu, L.; Zhang, Y.; Zhang, Y. Functionalization of multi-wall carbon nanotubes with silane and its reinforcement on polypropylene composites. Compos. Sci. Technol.
**2008**, 68, 1727–1733. [Google Scholar] [CrossRef] - Pantano, A.; Modica, G.; Cappello, F. Multiwalled carbon nanotube reinforced polymer composites. Mater. Sci. Eng. A
**2008**, 486, 222–227. [Google Scholar] [CrossRef] - Yamamoto, G.; Shirasu, K.; Nozaka, Y.; Wang, W.; Hashida, T. Microstructure–property relationships in pressureless-sintered carbon nanotube/alumina composites. Mater. Sci. Eng. A
**2014**, 617, 179–186. [Google Scholar] [CrossRef] - Nozaka, Y.; Wang, W.; Shirasu, K.; Yamamoto, G.; Hashida, T. Inclined slit-based pullout method for determining interfacial strength of multi-walled carbon nanotube-alumina composites. Carbon
**2014**, 78, 439–445. [Google Scholar] [CrossRef] - Peng, B.; Locascio, M.; Zapol, P.; Li, S.; Mielke, S.L.; Schatz, G.C.; Espinosa, H.D. Measurements of near-ultimate strength for multiwalled carbon nanotubes and irradiation-induced crosslinking improvements. Nat. Nanotechnol.
**2008**, 3, 626–631. [Google Scholar] [CrossRef] [PubMed] - Yamamoto, G.; Shirasu, K.; Hashida, T.; Takagi, T.; Suk, J.W.; An, J.; Piner, R.D.; Ruoff, R.S. Nanotube fracture during the failure of carbon nanotube/alumina composites. Carbon
**2011**, 49, 3709–3716. [Google Scholar] [CrossRef] - Yamamoto, G.; Suk, J.W.; An, J.; Piner, R.D.; Hashida, T.; Takagi, T.; Ruoff, R.S. The influence of nanoscale defects on the fracture of multi-walled carbon nanotubes under tensile loading. Diam. Relat. Mater.
**2010**, 19, 748–751. [Google Scholar] [CrossRef] - Shirasu, K.; Yamamoto, G.; Hashida, T. How do the mechanical properties of carbon nanotubes increase? An experimental evaluation and modeling of the engineering tensile strength of individual carbon nanotubes. Mater. Res. Express
**2019**, 6, 055047. [Google Scholar] [CrossRef] - Xia, Z.H.; Guduru, P.R.; Curtin, W.A. Enhancing mechanical properties of multiwall carbon nanotubes via sp
^{3}interwall bridging. Phys. Rev. Lett.**2007**, 98, 245501. [Google Scholar] [CrossRef][Green Version] - Byrne, E.M.; McCarthy, M.A.; Xia, Z.; Curtin, W.A. Multiwall nanotubes can be stronger than single wall nanotubes and implications for nanocomposite design. Phys. Rev. Lett.
**2009**, 103, 045502. [Google Scholar] [CrossRef][Green Version] - Plimpton, S. Fast parallel algorithms for short-range molecular dynamics. J. Comput. Phys.
**1995**, 117, 1–19. [Google Scholar] [CrossRef][Green Version] - Stuart, S.J.; Tutein, A.B.; Harrison, J.A. A reactive potential for hydrocarbons with intermolecular interactions. J. Chem. Phys.
**2000**, 112, 6472–6486. [Google Scholar] [CrossRef][Green Version] - Zhao, H.; Min, K.; Aluru, N.R. Size and chirality dependent elastic properties of graphene nanoribbons under uniaxial tension. Nano Lett.
**2009**, 9, 3012–3015. [Google Scholar] [CrossRef] - Choi, B.K.; Yoon, G.H.; Lee, S. Molecular dynamics studies of CNT-reinforced aluminum composites under uniaxial tensile loading. Compos. B Eng.
**2016**, 91, 119–125. [Google Scholar] [CrossRef] - Deb Nath, S.K.; Kim, S.G. Study of the nanomechanics of CNTs under tension by molecular dynamics simulation using different potentials. ISRN Condens. Matter Phys.
**2014**, 2014, 606017. [Google Scholar] [CrossRef] - Yamamoto, G.; Shirasu, K.; Nozaka, Y.; Sato, Y.; Takagi, T.; Hashida, T. Structure-property relationships in thermally-annealed multi-walled carbon nanotubes. Carbon
**2014**, 66, 219–226. [Google Scholar] [CrossRef] - Shenderova, O.A.; Brenner, D.W.; Omeltchenko, A.; Su, X.; Yang, L.H. Atomistic modeling of the fracture of polycrystalline diamond. Phys. Rev. B
**2000**, 61, 3877. [Google Scholar] [CrossRef][Green Version] - Thamaraikannan, S.; Pradhan, S.C. Atomistic study of carbon nanotubes: Effect of cut-off distance. In Proceedings of the TMS 2016 145th Annual Meeting & Exhibition, Music City Center, Nashville, TN, USA, 15–17 February 2016; Springer: Cham, Switzerland, 2016; pp. 293–300. [Google Scholar] [CrossRef]
- Jhon, Y.I.; Jhon, Y.M.; Yeom, G.Y.; Jhon, M.S. Orientation dependence of the fracture behavior of graphene. Carbon
**2014**, 66, 619–628. [Google Scholar] [CrossRef] - Currin, C.; Mitchell, T.; Morris, M.; Ylvisaker, D. A Bayesian Approach to the Design and Analysis of Computer Experiments; Oak Ridge National Laboratory: Oak Ridge, TN, USA, 1988. [Google Scholar]
- Shahriari, B.; Swersky, K.; Wang, Z.; Adams, R.P.; De Freitas, N. Taking the human out of the loop: A review of Bayesian optimization. Proc. IEEE
**2015**, 104, 148–175. [Google Scholar] [CrossRef][Green Version] - Sacks, J.; Welch, W.J.; Mitchell, T.J.; Wynn, H.P. Design and analysis of computer experiments. Stat. Sci.
**1989**, 4, 409–423. [Google Scholar] [CrossRef] - Jones, D.R.; Schonlau, M.; Welch, W.J. Efficient global optimization of expensive black-box functions. J. Glob. Optim.
**1998**, 13, 455–492. [Google Scholar] [CrossRef] - Holland, J.H. Adaptation in Natural and Artificial Systems: An Introductory Analysis with Applications to Biology, Control, and Artificial Intelligence; MIT Press: Cambridge, MA, USA, 1992. [Google Scholar] [CrossRef]
- Goldberg, D.E. Genetic algorithms in search. In Optimization, and Machine Learning; Addison Wesley Publishing Company: Boston, MA, USA, 1989. [Google Scholar]
- Deb, K. Multi-Objective Optimization Using Evolutionary Algorithms; John Wiley & Sons: Hoboken, NJ, USA, 2001. [Google Scholar]
- Michalewicz, Z. Genetic Algorithms + Data Structures = Evolution Programs; Springer Science & Business Media: Berlin, Germany, 2013. [Google Scholar]
- Fonseca, C.M.; Fleming, P.J. Genetic algorithms for multiobjective optimization: Formulation, discussion and generalization. In Proceedings of the Fifth International Conference on Genetic Algorithms, Urbana-Champaign, IL, USA, 17–21 July 1993; pp. 416–423. [Google Scholar]
- Baker, J.E. Adaptive selection methods for genetic algorithms. In Proceedings of the International Conference on Genetic Algorithms and their Applications, Pittsburg, PA, USA, 24–26 July 1985; pp. 101–111. [Google Scholar] [CrossRef]
- Eshelman, L.J.; Schaffer, J.D. Real-coded genetic algorithms and interval-schemata. FOGA
**1993**, 2, 187–202. [Google Scholar] [CrossRef] - Qian, J.; Nguyen, N.P.; Oya, Y.; Kikugawa, G.; Okabe, T.; Huang, Y.; Ohuchi, F.S. Introducing self-organized maps (SOM) as a visualization tool for materials research and education. Results Mater.
**2019**, 4, 100020. [Google Scholar] [CrossRef] - Kohonen, T. The self-organizing map. Proc. IEEE
**1990**, 78, 1464–1480. [Google Scholar] [CrossRef] - Viscovery. Available online: https://www.viscovery.net/somine/ (accessed on 1 October 2020).
- Kohonen, T.; Kaski, S.; Lagus, K.; Salojarvi, J.; Honkela, J.; Paatero, V.; Saarela, A. Self organization of a massive document collection. IEEE Trans. Neural Netw.
**2000**, 11, 574–585. [Google Scholar] [CrossRef] [PubMed][Green Version] - Natsuki, T.; Tantrakarn, K.; Endo, M. Effects of carbon nanotube structures on mechanical properties. Appl. Phys. A
**2004**, 79, 117–124. [Google Scholar] [CrossRef] - Liu, F.; Ming, P.; Li, J. Ab initio calculation of ideal strength and phonon instability of graphene under tension. Phys. Rev. B
**2007**, 76, 064120. [Google Scholar] [CrossRef][Green Version] - Pregler, S.K.; Sinnott, S.B. Molecular dynamics simulations of electron and ion beam irradiation of multiwalled carbon nanotubes: The effects on failure by inner tube sliding. Phys. Rev. B
**2006**, 73, 224106. [Google Scholar] [CrossRef]

**Figure 1.**Schematic diagram of the computational model. (

**a**) Entire 2WCNT with Frenkel-pair crosslinks and distortions on the wall with a half front slice on the left side, where the two red parts (on the outermost wall) indicate the regions of load application during the tensile test and are named fixed parts. The blue color (including all inner walls) represents the parts where atoms can move freely, and are thus named mobile parts; (

**b**) Magnified view of the middle mobile part of 2WCNT; (

**c**) Front slice of (

**b**) showing randomly distributed crosslinks; (

**d**,

**e**) Structure of Frenkel-pair crosslink. Light blue balls represent carbon atoms on the inner walls, and yellow balls are atoms on the outer walls.

**Figure 2.**Flowchart of the optimization procedure. (

**a**) Bayesian optimization; (

**b**) genetic algorithm.

**Figure 3.**Strength results of the machine learning–predicted structure with respect to the repetition of the prediction procedure. Error bar shows the maximum and minimum values obtained from the three repetitions of calculations.

**Figure 4.**Fracture patterns of the zigzag-type 5WCNTs assigned with different crosslink densities. (

**a**) “Sword-in-sheath” fracture on the 0.5% crosslink model (in every wall) with nominal strength of 47 GPa; (

**b**) “Sword-and-sheath” fracture on the 0.75% crosslink model with nominal strength of 50 GPa; (

**c**,

**d**) “Near-clean-break” and “clean-break” fracture on the 1.5% crosslink model with nominal strength of 53 GPa and 52 GPa, respectively.

**Figure 5.**SOM results including the cluster map and heat map. (

**a**) Cluster map with 7 clusters; (

**b**) Heat map of nominal tensile strength: values range from 20.1 GPa to 62.6 GPa; (

**c**) Heat map of nominal Young’s modulus: values range from 147 GPa to 694 GPa; (

**d**–

**f**) Heat map of chirality, diameter, and number of walls, respectively; (

**g**–

**j**) Heat maps of crosslink density 1–4, where crosslink density 1 is the density corresponding to the innermost wall, and crosslink density 4 is the density corresponding to the outermost wall.

**Figure 6.**Fracture behavior difference between zigzag-type and armchair-type 2WCNTs. (

**a1**) Approximately 30° fracture for armchair-type CNT; (

**b1**) Nearly linear fracture for zigzag-type tube; (

**a2**,

**b2**) Atom arrangement of armchair-type CNT and zigzag-type CNT, respectively.

**Table 1.**Detailed information for the representative values in Figure 4. “Crosslink density 1” through “Crosslink density 4” represent the crosslink densities between each adjacent wall from the inner tube to the outer tube. The average value is given, and the range is indicated in parentheses.

Model | Outer Diameter (Å) | Number of Walls | Chirality | Crosslink Density 1 (%) | Crosslink Density 2 (%) | Crosslink Density 3 (%) | Crosslink Density 4 (%) | Nominal Tensile Strength (GPa) |
---|---|---|---|---|---|---|---|---|

① | 101.70 | 5 | Armchair | 0.01 (0.01–0.01) | 2.32 (2.31–2.32) | 2.36 (2.35–2.37) | 2.26 (2.25–2.28) | 27.79 (27.53–28.04) |

② | 44.75 | 5 | Armchair | 0.91 (0.89–0.92) | 0.75 (0.74–0.77) | 0.97 (0.95–0.97) | 1.38 (1.35–1.41) | 60.53 (57.60–62.81) |

③ | 44.62 | 5 | Zigzag | 0.02 (0.02–0.02) | 0.83 (0.81–0.85) | 0.05 (0.04–0.05) | 1.70 (1.69–1.71) | 37.58 (36.28–40.02) |

④ | 43.39 | 5 | Armchair | 2.85 (2.81–2.90) | 1.19 (1.18–1.21) | 1.47 (1.45–1.48) | 1.83 (1.81–1.84) | 57.19 (55.80–59.88) |

⑤ | 43.39 | 5 | Armchair | 0.22 (0.20–0.23) | 0.44 (0.44–0.45) | 2.11 (2.10–2.12) | 1.20 (1.20–1.21) | 60.03 (56.62–62.12) |

⑥ | 43.39 | 5 | Armchair | 0.05 (0.04–0.05) | 2.03 (2.01–2.05) | 1.32 (1.30–1.35) | 1.32 (1.31–1.33) | 58.50 (54.77–61.42) |

⑦ | 43.39 | 5 | Armchair | 1.98 (1.97–2.00) | 0.84 (0.82–0.86) | 0.59 (0.57–0.60) | 1.01 (1.00–1.03) | 58.26 (56.25–59.52) |

⑧ | 43.39 | 5 | Armchair | 0.90 (0.89–0.92) | 1.39 (1.36–1.41) | 1.40 (1.40–1.41) | 1.25 (1.23–1.28) | 58.83 (58.02–60.26) |

Publisher’s Note: MDPI stays neutral with regard to jurisdictional claims in published maps and institutional affiliations. |

© 2020 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).

## Share and Cite

**MDPI and ACS Style**

Xiang, Y.; Shimoyama, K.; Shirasu, K.; Yamamoto, G. Machine Learning-Assisted High-Throughput Molecular Dynamics Simulation of High-Mechanical Performance Carbon Nanotube Structure. *Nanomaterials* **2020**, *10*, 2459.
https://doi.org/10.3390/nano10122459

**AMA Style**

Xiang Y, Shimoyama K, Shirasu K, Yamamoto G. Machine Learning-Assisted High-Throughput Molecular Dynamics Simulation of High-Mechanical Performance Carbon Nanotube Structure. *Nanomaterials*. 2020; 10(12):2459.
https://doi.org/10.3390/nano10122459

**Chicago/Turabian Style**

Xiang, Yi, Koji Shimoyama, Keiichi Shirasu, and Go Yamamoto. 2020. "Machine Learning-Assisted High-Throughput Molecular Dynamics Simulation of High-Mechanical Performance Carbon Nanotube Structure" *Nanomaterials* 10, no. 12: 2459.
https://doi.org/10.3390/nano10122459